The International Journal Of Engineering And Science (IJES)||Volume||2 ||Issue|| 5 ||Pages|| 40-45||2013||ISSN(e): 2319 – 1813 ISSN(p): 2319 – 1805www.theijes.com The IJES Page 40Experimental Investigation on Silica Fume aspartial Replacementof Cement in High Performance Concrete1,T.Shanmugapriya , 2,Dr.R.N.Uma1,Department of Civil Engineering,Sri Ramakrishna Institute of Technology, Coimbatore -10, India.2,Department of Civil Engineering,Sri Ramakrishna Institute of Technology, Coimbatore -10, India.-----------------------------------------------------ABSTRACT-----------------------------------------------------With increased environmental awareness and its potential hazardous effects, utilization of industrial byproductshas become an attractive alternative to disposal. Silica fume(SF), which is byproduct of the smelting process inthe silicon and ferrosilicon industry. Silica fume is very effective in the design and development of highperformance concrete.This paper presents the results of an experimental investigations carried out to findthe suitability of silica fume in High Performance concrete. The concrete used in this investigation wasproportioned to target a mean strength of 60 MPa and designed as per ACI 211.4R-08.The water binder ratio(W/B) adopted was 0.32 and the Super Plasticizer used was CONPLAST SP 430.Specimens such as cubes,beams and cylinders were cast for various mix proportions and tested at the age of 7,14and 28 days. Theinvestigation revealed that the partial replacement of cement by silica fume will develop compressive strength,flexure strength and split tensile strength sufficient for construction purposes. The optimum dosage of silicafume found to be 7.5% (by weight), when used as partial replacement of ordinary Portland cement .Its use willlead to a reduction in cement quantity required for construction purposes and hence sustainability in theconstruction industry as well as economic construction.KEY WORDS: Compressive strength,Flexure strength, High Performance Concrete, Silica fume,Split Tensilestrength--------------------------------------------------------------------------------------------------------------------------------------Date of Submission: 25,May ,2013 Date of Publication: 5.June,2013--------------------------------------------------------------------------------------------------------------------------------------I. INTRODUCTIONHigh Performance Concrete (HPC) has been developed over the last two decades, and was primarilyintroduced through private sector architectural design and construction such as high rise buildings and parkinggarages. HPC is used for concrete mixtures, which possess high workability, high strength, high modulus ofelasticity, high density, high dimensional stability, low permeability and resistance to chemical attack.According to ACI “High Performance Concrete is defined as concrete whichmeets special performance anduniformity requirementsthat cannot always be achieved routinely by using conventional materials and normalmixing, placing and curing practices”.The supplementary cementitiousmaterials (SCMs) such as silica fume, fly ash and ground granulatedblast furnace slag are more commonly used mineral admixtures in the development of HPC mixes.Theygenerally used to resist compressive forces and also due to its pozzolanicaction the properties of HighPerformance Concreteviz, workability, durability, strength, resistance to cracks and permeability can beimproved.Silica Fume is most commonly used supplementarycementitous materials used in the developmentof High Performance Concrete.Silica fume (SF) is a byproduct of the smelting process in the silicon andferrosilicon industry. It is also known as micro silica,condensed silica fume, volatilized silica or silica dust.Silica fume colour is either premium white or grey. Silica Fume consists of very fine vitreous particles with asurface area between 13,000 and 30,000m2/kg. Its particles are approximately 100 times smaller than theaverage cement particle. Because of its extreme fineness and high silica content, silica fume is a highly effectivepozzolanicmaterial. Silica fume is used in concrete to improve its properties. It has been found that silica fumeimproves compressive strength, bond strength, and abrasion resistance; reduces permeability; and thereforehelps in protecting reinforcing steel from corrosion.When Silica fume are incorporated to concrete, the silicapresent in these materials react with the calcium hydroxide released during the hydration of cement and formsadditional calcium silicate hydrate (C – S – H ), which improve durability and the mechanical properties ofconcrete.
Experimental Investigation On Silica…www.theijes.com The IJES Page 41High compressive strength is generally the first property associated with silica fume concrete. Theaddition of silica fume to a concrete mix will increase the strength of that mix by between 30% and 100%depending on the type of mix, type of cement, amount of silica fume, use of plasticizers, aggregate types andcuring regimes. Silica fume concrete is very susceptible to temperature variations during the hardeningprocess. The optimum silica fume content to achieve higher strengths seems to range between 15 and20%.There are three mechanisms namely (i)Strength enhancement by pore sizerefinement and matrixdensification, (ii) Strength enhancement by reduction in content of CH and (iii) Strength enhancement bycement paste- aggregateinterfacial refinement are believed to be responsible for the strength development ofconcrete and mortars containing silica fume.High range water reducing admixtures (Super plasticizer) is used as a part of chemical admixturesinHigh Performance Concrete to produce better workability and high strengths. The brief literature on the studyhas been presented in following text.The influence of silica fume in replacement of cement on physicalproperties and resistance to sulphate attack, freezing and thawing, and alkali silica reactivity and the maximum28 days compressive strength was obtained at 15% silica fume replacement level, at a W/C ratio of 0.35 withvariable dosages of HRWRA.High PerformanceConcrete with silica fume at a constant water binder ratio(w/b) of 0.34 and replacement percentages of 0 to 25, with varying dosages of HRWRA increases thecompressive strength, the optimum percentage was obtained at 15% replacement level. Developing HighPerformance with a better understanding of the isolated contributions of silica fume on concrete over a widerange of w/c ratio ranging from 0.26 to 0.42 and cement replacement percentages from 0 to 30. The mainobjective of this investigation is to minimize the usage of cement content to some proportion in the HighPerformance Concrete. This present work is to study various properties namely compressive strength, SplitTensile Strength and Flexure strength of M60 grade HPC mixes incorporating different percentages silica fumeby weight of cement along with SulphonatedNapthalenebased super plasticizer (CONPLAST SP 430).II. EXPERIMENTAL PROGRAMMEThe Experimental Programme was designed to compare the mechanical properties of HighPerformance Concretewith M60 grade of concrete with different replacement levels of ordinary Portland cement53 grade with silica fume. The replacement levels of cement by silicafume are selected as 2.5%, 5%, 7.5%,10%, and12.5% .The specimens of Cubespecimen of size 150 x 150 x 150 mm,Cylinder specimen of size 150mm diameter and 300 mm height and Beam specimen of size 100 x100 x 500 mm were preparedwith andwithout silica fume.2.1 Materials UsedCement: Ordinary Portland cement of 53 Grade was used and the specific gravity of cement was foundto be 3.15.Silica Fume (Grade 920 D): Obtained from ELKEM South Asia Pvt.Ltd.Mumbai, was named Elkem – microsilica 920 D conforming to ASTM C1240.The physical and chemical properties of cement and silica fume aregiven in Table.1Table 1.Physicaland chemicalProperties of cement and silica fumeProperties OPC Silica fumePhysicalSpecific gravity 3.15 2.2Specific area cm2/gm 3250 1800000ChemicalSilicon di oxide(SiO2) 20.3 89.5Aluminium oxide(Al2O3) 6.3 1.2Iron Oxide(Fe2O3) 3.12 2Calcium Oxide(CaO) 63.6 0.2-0.8Magnesium Oxide(MgO) 1.6 0.2-0.8Sodium Oxide(Na2O) 0.4 0.5-1.2Potassium Oxide(K2O) 0.51 -Loss of Ignition 1.13 3
Experimental Investigation On Silica…www.theijes.com The IJES Page 42Fine Aggregate: River sand having bulk density 1720 kg/m3was used and the specific gravity was found to be2.56 .Sieve analysis results are shown in Table. 2Table 2 Sieve analysis of River sandSieve Size River sand% Passing4.75mm 982.36mm 961.18mm 78600µm 51300 µm 26150 µm 7Coarse Aggregate: Crushed angular aggregate with maximum grain size of 12.5mm and down graded was usedand having bulk density 1691kg/m3. The specific gravity and fineness modulus was found to be 2.78 and 2.75respectively.Super plasticizer: CONPLAST SP 430 was used as water reducing agent to achieve the required workability. Itis based on SulphonatedNapthalene polymers complies with IS 9103:1999 and ASTM C 494 type F as a highrange water reducing admixture. It is a brown liquid instantly dispensable in water.Water: Fresh portable water, which is free from acid and organic substance, was used for mixing the concrete.2.2 Mix ProportioningConcrete mix design in this investigation was designed as per the guidelines specified in ACI 211.4R-08 - “Guide for selecting proportions for high strength concrete with portland cement and other cementationsmaterials”. Six concrete mixtures with different proportions of silica fume ranging from 0% (for the controlmix) to 12.5%.The mix proportions were calculated and presented in Table. 3Table 3.Mixproportion for High Performance ConcreteMaterialsCement(%)SilicaFume(%)Cement(kg/m3)SilicaFume(kg/m3)Fineaggregate(kg/m3)Coarseaggregate(kg/m3)W/BRatioC 100 0 551.87 - 672 1149.80.32SF 2.5% 97.5 2.5 532.35 13.8 672 1149.8SF 5% 95 5 512.51 27.59 672 1149.8SF 7.5% 92.5 7.5 492.66 41.39 672 1149.8SF 10% 90 10 472.5 55.19 672 1149.8SF 12.5% 87.5 12.5 453.6 68.98 672 1149.82.3 Casting and curing of Test specimens:The specimen of standard cube, Cylinder and beams were used to determine the compressive strengthSplit tensile and flexural strength of concrete. Three specimens were tested for 7, 14 & 28 days with eachproportion of Silica fume replacement. For each measured quantities of coarse aggregate and fine aggregate wasspread in a pan, the ordinary Portland cement (53 Grade) and silica fume were spread out over it, water wasmeasured by considering the water binder ratio as 0.32 and weight of super plasticizer(CONPLAST SP 430)was estimated as 1.2 % of weight of binder. The exact quantity of water and super plasticizer was added. Theconcrete was thoroughly mixed until it achievedhomogeneousand uniform consistency. The fresh concrete wascast in cube, cylinder and beam moulds, and was compacted by table vibrator.All freshly cast specimens wereleft in the moulds for 24 hours before being de moulded. The de mouldedspecimens were cured in water for7,14&28 days, were air dried and then tested for its compressivestrength, Split tensile strength and flexuralstrength as per Indian standards.
Experimental Investigation On Silica…www.theijes.com The IJES Page 43III. RESULTS AND DISCUSSIONSCompressive strength of concrete:The test was carried out conforming to IS 516-1959 to obtain compressive strength of concrete at theage of 7, 14 and 28 days. The cubes were tested using Compression Testing Machine (CTM) of capacity2000KN. The results are presented in Figure 1Fig. 1-Compressive Strength of High Performance ConcreteWithvarious proportions of Silica fumeFig. 1 shows the variation of compressive strength with silica fume replacement percentage. There is asignificant improvement in the compressive strength of concrete because of the high pozzolanic nature of thesilica fume and void filling ability. The compressive strength with replacement of cement by silica fume wasincreased 0% to 7.5% and then decreased. Hence the optimum silica fume was 7.5%. The optimum silica fumereplacement percentage for obtaining maximum 28-day strength of concrete ranged from 5% to 20%. Themaximum value of compressive strength was obtained as 65.33MPa at 7.5% replacement of silica fume.3.2Split Tensile Strength of ConcreteThe test was carried out conforming to IS 516-1959 to obtain split tensile strength of concrete at theage of 7, 14 and 28 days. The cylinders were tested using Compression Testing Machine (CTM) of capacity2000KN. The results are presented in Figure 2.Fig 2.Split tensile Strength of High Performance ConcreteWithvarious proportions of Silica fume
Experimental Investigation On Silica…www.theijes.com The IJES Page 44The Split tensile strength of the High Performance Concrete increases with the increase in percentageof Silica Fume. The partial replacement of 7.5% Silica fume is found to be optimum.High PerformanceConcrete at the age of 28 days with partial replacement of 7.5% cement by silica fume showed20%greaterSplittensile Strengththan conventional concrete respectively.3.3.Flexural strength of concrete:The test was carried out conforming to IS 516-1959 to obtain Flexural strength of concrete at the age of 7,14 and28 days. The beams were tested using Flexure Testing Machine (FTM) of capacity 100KN. The results arepresented in Figure.3Fig 3.Flexural Strength of High Performance ConcreteWithvarious proportions of Silica fumeThe flexural strength at the age of 28 days of silica fume concrete continuously increased with respectof to controlled concrete and reached maximum value of 7.5% replacement level.High Performance Concrete atthe age of 28 days with partial replacement of 7.5% cement by silica fume showed 23%greaterflexuralStrengththan conventional concrete. It can be concluded that the ultra – fine silica fume particles, which consistsmainly of amorphous silica, enhance the concrete strength by both pozzolanic and physical actions.IV. CONCLUSIONS:High performance concrete produced from cement replacement upto 7.5% silica fume leads to increasein compressive strength, split tensile and Flexure strength of concrete. Beyond 7.5 %there is a decrease incompressive strength, split tensile and Flexure strength of concrete.The compressive strength mainly depends onthe percentage of silica fume because of its high pozzolanic nature to form more densely packed C-S-H gel.HighPerformance Concrete with silica fume can be effectively used in high rise buildings since high early strength isrequired, and the construction period can be reduced.The percentage of increase in the compressive strength is15%, Split tensile strength is 20% andthe flexure strength is 23% at the age of 28 days by replacing 7.5% ofcement by silica fume.The optimum percentage of replacement of cement by silica fume is7.5%REFERENCES: Sensale GR., Strength development of concrete with rice husk ash, Cement and Concrete Composites,28(2), 2006, 158-160. Mohammad IqbalKhana and RafatSiddiqueb, Utilization of silica fume in concrete: Review of durability properties, Resources,Conservation and Recycling, 2011, 57, 30–35 Igarashi S, Watanabe A and Kawamura M., Evaluation of capillary pore size characteristics in high-strength concrete at earlyages. Cement and Concrete Research, 35(3), 2005, 513- 519. Bhanja,s. and Sengupta,B.(2002).”Investigations on the composite structure ofsilica fume concrete using statisticalmethods”,Cement and Concrete Research,Vol.32, pp.1391-1394. Aitcin, P.C., and Laplante, P. (1990),“Long-term compressive strength of silicafume concrete”, Journal of Materials inCivilEngineering, Vol. 2, No. 3, pp. 164-170. Feldman, R.F., Cheng-yi, H. (1985),"Properties of Portland cement silica fumepastes. II mechanical properties", Cement andConcrete Research, Vol. 15 No.6, pp.943. Yogendran V, Langan BW, Haque M and Ward MA.Silica on high strength concrete, ACI MaterialJournal, No. 2, 84(1987) 124– 129.
Experimental Investigation On Silica…www.theijes.com The IJES Page 45 Bhanja S, Sengupta B. Optimum silica fume content and its mode of action on concrete, ACI MaterialsJournal, September –October 2003, pp. 407 – 712. ACI Committee 211.4R.93, “Guide forSelecting properties for High StrengthConcrete with Portland Cement and Fly ash”ACImanual of concrete Practice, 2001. S.A. Khedr, M.N and Abou-Zeid, Characteristics of silica-fume concrete, J. Mater. Civ. Eng. ASCE 6 (3), 1994, 357–375.